Chip out a “U” shaped slot as per the drawings shown above and depending on the wall to slab interface configuration such that the bottom corner of the slot is cen- tered over the construction joint. The slot is to be 1” (25 mm) wide by at least 2” - 3” (50 - 75 mm) deep. A “V” shaped slot is not acceptable. The slot may be saw cut instead of chipped but ensure that the slot is dovetailed or otherwise shaped such that there will be mechanical interlock of mate- rials placed into the slot at a later stage.
In area of greatest water flow, drill hole or cavity 0.5” (13 mm) deeper into slot and over the joint to accommodate a bleeder hose. A bleeder hose is a minimum 1.5 foot (0.5 m) length of smooth surfaced, fairly rigid tubing. Its purpose is to relieve the water pressure while crack/joint is being repaired.
Remove all loose materials within the slot and to 6” (150 mm) on either side of slot. Clean, profile (ICRI CSP-3) and saturate this area with water. Allow water to soak into concrete and then remove all surface water.
Place one end of bleeder hose into the hole or cavity and, while holding hose steady, apply Xypex Patch’n Plug to the slot around the hose. Approximately two to four applica- tions of Patch’n Plug may be necessary to secure the hose in place and embed the tubing completely up to surface level.
To stop active water flow apply Xypex Patch’n Plug to half the depth of remaining slot area. Patch’n Plug is mixed by adding one part clean water to 3.5 parts Patch’n Plug powder by volume. If slot has dried out before Patch’n Plug application, it should be re-wetted. Remove bleeder hose and pack hole with Xypex Patch’n Plug to stop all active water flow.
Apply a slurry coat of Xypex Concentrate at a cover- age of 1.5 lb./sq. yd. (0.8 kg/m2) in the slot, over the Patch’n
Plug, and to 6” (150 mm) up the wall and onto the slab away from the slot. Application may be performed by brush or gloved hand.
While slurry coat is still tacky, fill slot to surface with Xypex Concentrate Dry-Pac mixed in the following pro- portions: one part clean water to six parts Concentrate by volume. Blend Dry-Pac by trowel for 10 - 15 seconds only (lumps should be present in the mixture). Apply Dry-Pac by gloved hand, and then compress it tightly using a pneumatic packing device or a hammer and block.
Wet Dry-Pac surface lightly with water, then apply a slurry coat of Xypex Concentrate at coverage of 1.5 lb./sq. yd. (0.8 kg/m2) over the repaired area and to 6” (150 mm) up the wall and onto the slab away from the slot.
Cure by keeping moist using Gamma Cure and/or by fog spraying periodically with water for two to three days. Open to water contact per Xypex Coatings guidelines.
When early exposure to water is required:
1. In Step 7 – replace the top 1⁄4” - 1⁄2” (6 - 12 mm)
of Xypex Concentrate Dry-Pac with Xypex Patch’n Plug.
2. Step 8 and Step 9 – eliminate.